Research Article  Open Access
Tuning Electronic Structures of BN and C DoubleWall HeteroNanotubes
Abstract
First principle calculations based on density functional theory with the generalized gradient approximation were carried out to investigate the energetic and electronic properties of carbon and boron nitride doublewall heteronanotubes (C/BNDWHNTs) with different chirality and size, including an armchair (, ) carbon nanotube (CNT) enclosed in (, ) boron nitride nanotube (BNNT) and a zigzag (, 0) CNT enclosed in (, 0) BNNT. The electronic structure of these DWHNTs under a transverse electric field was also investigated. The ability to tune the band gap with changing the intertube distance () and imposing an external electric field () of zigzag DWHNTs provides the possibility for future electronic and electrooptic nanodevice applications.
1. Introduction
Carbon nanotubes (CNTs) play a very important role in nanodevice applications due to their novel properties. by comparison with CNTs, boron nitride nanotubes (BNNTs) are formed with similar structures, however, of very distinctive properties [1]. Of similar crystalline structure, hexagonal boron nitride (hBN) has been considered as a potential substrate material for graphene [1, 2]. Recently, the structures of bilayer and trilayer graphene/hBN have been reported with tunable band gaps for electronic device applications [3–5].
Hexagonal boron nitride shares similar crystalline structure with graphene, and it is slightly latticemismatched from graphene by about 1.5%, which implies that it is possible to form heteronanostructures. BNNTs’ growth on CNT has successfully been applied to nanowires [6]. Several studies have also been conducted on BNcoated CNTs [7, 8]. The BNNT around the CNTs effectively helps to protect them and makes them more stable; for example, oxidation degradation of CNTs is reduced by coating with BNNTs, and the thermal stability of CNT@BNNTs is far superior to CNTs [9].
An efficient way to modify the band gap of nanotubes is to apply an external electric field [10]. The response of the nanotube to is of interest for studying its future application, such as that in logic gates, static memory cells, and sensor devices [11–13]. Ab initio calculation showed that band gaps of both CNTs and BNNTs can be greatly reduced by a transverse electric filed [14, 15]. An intriguing question to answer is whether external electric fields can also be an efficient way to modulate the electronic properties of C/BNDWHNTs.
However, a firstprinciples study on the stability as well as the electronic properties modulated with and of C/BNDWHNTs is not available. To fill the deficiency, in this work, we performed a series of firstprinciples calculations to study the coaxial CNT@BNNT and to examine the electric field shielding effect of BNNT on the inside CNT. We calculated the band structures of coaxial CNT@BNNT consisting of armchair and zigzag CNT cores and BNNT sheaths, focusing on the band structure variations with and . The relative insensitivity of armchair CNT@BNNT to , at least for the few cases considered here, suggests that zigzag CNT@BNNT would be a suitable candidate for doublewall heteronanotubes devices.
2. Calculation Methods
The geometric structure optimization and calculation of the related electrical properties of the CNT@BNNT with no were conducted using SIESTA [16, 17] and adopted normconserving nonlocal pseudopotentials for the atomic core. The Perdew, Burke, and Ernzerhof (PBE) form generalized gradient approximation (GGA) corrections were employed for the exchangecorrelation potential energy [18]. The atomic orbital basis set employed throughout was doubleζ plus polarization functions (DZP). Periodic boundary condition along the axis was employed for nanotubes. Brillouin zones were sampled by a set of points grid (1 × 1 × 8) according to the MonkhorstPack approximation [19].
When electric field was imposed, the calculation was using density functional theory available in DMol3 code [20, 21]. The PBE function [22] of GGA was used to calculate the exchangecorrelation potential energy, the all electron approach was used, and the orbit population parameter smearing was set at 0.0005 a.u.
Our models were constructed within a tetragonal super cell with lattice constants of and equaling 40 Å to avoid the interaction between two adjacent nanotubes and , the lattice constant in direction along the tube axis, equaling onedimensional (1D) lattice parameter of the nanotubes. The tube was taken along the direction and the circular cross section was lying in the () plane. Both the CNT and BNNTs structures were fully optimized until the force on each atom was less than 0.005 eV Å^{−1} during relaxation.
The van der Waals interactions are very important in twodimensional materials [23], especially in layered structures. The van der Waals force has obvious effect on the adsorption energy and adsorption position and height [24–26]. In this paper, the distances of the CNT and BNNT are fixed, and the optimization does not change the C/BNDWHNTs structures. The van der Waals interactions could increase the value of , but they should not affect the electronic properties of C/BNDWHNTs [10].
3. Results and Discussion
Two types of C/BNDWHNTs were investigated, zigzag and armchair. The zigzag C/BNDWHNTs are studies that include CNT(, 0)@BNNT(, 0) (, ). The armchair C/BNDWHNTs considered are CNT(, )@BNNT(, ) (, ). Figure 1(a) gives an illustration of the coaxial armchair CNT(5, 5) inside armchair BNNT(10, 10), the left (right) panel for the top (lateral) view of the initial structure.
(a)
(b)
The calculated covalent bond lengths of the various C/BNDWHNTs in the fully optimized structures are listed in Table 1. For any C/BNDWHNTs, we define the binding energy per atom as , where , , and are the energy of isolated carbon, boron, and nitride atoms, respectively. is the total energy of a C/BNDWHNT, is the number of C atoms, and is the number of B and N atoms. The formation energy of each C/BNDWHNT is also calculated, in which the and are the binding energy of free standing CNT and BNNT, respectively.
(a)  
 
(b)  
 
(c)  

The stability of C/BNDWHNTs is determined by the interaction force between the inner and outer nanotubes, as shown in Table 1. The formation energy varying with was plotted in Figure 1(b). When = ~2.60 Å, is positive, which means the free standing CNT and BNNT are favorite in energy. When = ~3.5 Å, the armchair C/BNDWHNTs have the lowest binding energy and formation energy, meaning that the armchair C/BNDWHNTs at = ~3.5 Å are more possible to exist. This result is in agreement with the literature [27], in which Yuan and Liew have studied the coaxial CNT@BNNT nanocables and found that the optimal intertube distances between inner C tube and the outer BN are about 3.5 Å for armchair nanocables.
The distance of the armchair C/BNDWHNTs can be approximately evaluated by the expression as ; here and are the bond lengths of outer BNNT and inner CNT, respectively. Let Å; the possible stable structures are CNT(, )@BNNT(, ) (), for example, CNT(5, 5)@BNNT(10, 10), CNT(6, 6)@BNNT(11, 11), and CNT(7, 7)@BNNT(12, 12) DWHNTs (see Table 1(a)). Taking the armchair CNT(5, 5)@BNNT(, ) () nanotubes as examples, the covalent bond lengths in the fully optimized CNT and BNNT are 1.43 and 1.45 Å, respectively. When = ~2.60 Å, the bond length of inner CNT was suppressed to 1.385 Å and the bond length of outer BNNT was extended to 1.540 Å in the perpendicular direction. This result indicates the occurrence of greater repulsive interactions between the inner CNT and the outer BNNT.
The calculated covalent bond lengths of the various zigzag DWHNTs in fully optimized structures are listed in Table 1(b). When = ~3.6 Å, the zigzag C/BNDWHNTs have the lowest binding energy and formation energy. It means that the C/BNDWHNTs at = ~3.6 Å are more possible to exist. For zigzag configurations, the distance is as follows: (; letting Å, the possible stable structures are CNT(, 0)@BNNT() (), for example, CNT(6, 0)@BNNT(15, 0), CNT(7, 0)@BNNT(16, 0) DWHNTs.
The calculated band structures of C/BNDWHNTs are shown in Figure 2. The armchair C/BNDWHNTs are metallic, with the lowest conduction band and the highest valence band crossing over the Fermi level at ~2/3 along direction in reciprocal space. The electric band structure near the Femi level is very similar to the CNTs because the lowest conduction band and the highest valence band are determined by the carbon atoms. We also found that changing cannot be an efficient way to open the band gap for armchair C/BNDWHNTs.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
(h)
(i)
The calculated band gaps () of the singlewall CNT(, 0) are 0.19, 0.58, 0.04, 0.78, and 0.87 eV for , respectively, which are consistent with results of similar studies [28]. For the zigzag DWHNTs, affects the band gap of C/BNDWHNTs. A different size CNT(7, 0) was considered as the inner tube of the zigzag C/BNDWHNTs. The calculated band gaps are listed in Table 1(b). All the zigzag CNT(7, 0)@BNNT structures are found to be direct gap semiconductors with both the valence band top and conduction band bottom at the Γ point. In Figure 3(a), analysis of the PDOS of CNT(7, 0)@BNNT indicated that p orbitals of the carbon atoms dominate the band near Femi level. However, for CNT(7, 0)@BNNT(14, 0), the p orbitals of the nitrogen atoms have a contribution to the bands near the Femi level, which also proved the stronger interaction when the strayed from ~3.6 Å. Figure 3(b) shows the DOS of CNT(7, 0)@BNNT(14, 0) and CNT(7, 0)@BNNT(16, 0) DWHNTs. The band gap of CNT(7, 0)@BNNT(14, 0) became small when comparing with the CNT(7, 0)@BNNT(16, 0) during the stronger intertube interactions.
(a)
(b)
After the CNTs were encapsulated into the BNNT, for the stable structure such as CNT(5, 5)@BNNT(10, 10), their geometries changed little. To study the effect of the transverse electric field on the electronic structure of the nanotubes, F along y direction (perpendicular to the tube axis) was imposed. We first examined the electronic properties of the CNT(5, 5) under an electronic field (see Figure 4(a)). The CNT(5, 5) remains semimetallic with an enhancement of density of states around the Fermi level with increasing the eternal electrical field. Two linear bands became flat (localized) around the Femi level in CNT(5, 5) with increasing field strengths. It can therefore be inferred that the conductance will be greatly enhanced. And the results were well consistent with the literature [29]. The calculated values of the band structures for the armchair CNT(5, 5)@BNNT(10, 10) at , 0.1 and 0.15 V/Å are presented in Figure 4(b). There is no distinct difference between the electronic structures of the CNT(5, 5)@BNNT(10, 10) under different transverse electric fields. It shows that the transverse field does not affect the electric structures evidently. Whereas the band structures for CNT(5, 5) under and V/Å show a striking contrast, the band structures for the CNT(5, 5)@BNNT(10, 10) under and V/Å are quite similar. The same phenomenon has been found for CNT (6, 6)@BNNT(10, 10) and CNT (7, 7)@BNNT(12, 12) DWHNTs when is smaller than critical (here is a boundary when , the band structure of armchair CNT@BNNT would change abruptly, when , and the band structure of armchair CNT@BNNT would keep original shape). See the results in Table 1(c); both CNT and BNNT singlewalled nanotubes experience large structural changes after geometric optimization with increasing . When V/Å, optimized CNT(5, 5) was distortion.
(a)
(b)
However, with increasing , the DOS of the CNT@BNNT is not a simple superposition of the DOS for the individual CNT and pristine BNNT under . The peak heights for several particular states on the DOS are moderately strengthened or weakened due to the tubetube interaction. To explore the origin of this phenomenon, the PDOS for C, B, and N in pristine CNT(5, 5), BNNT(10, 10), and CNT(5, 5)@BNNT(10, 10) under electric fields and 0.25 V/Å was plotted, respectively, as shown in Figure 5. The calculated PDOS indicates that the states of carbon atoms contribute mainly to the energy levels near the Femi level. The states of boron and nitrogen in pristine BNNT are very sensitive to the . However, the change is not obvious in the heterostructure, which maybe caused by the effect of the tubetube interaction.
(a) V/Å
(b) V/Å
(c) V/Å
(d) V/Å
We also examined the electronic properties of the zigzag CNT (7, 0)@BNNT(16, 0) and CNT(10, 0)@BNNT(18, 0) under an electronic field. We found that with increasing the band gap of zigzag CNT (7, 0)@BNNT(16, 0) decreases gradually, and the phenomena are similar to the singlewall CNT (7, 0) under an electronic field. Though the band structure of zigzag CNT(10, 0)@BNNT(18, 0) also decreases gradually with increasing , it is different from the singlewall CNT(10, 0), because of the increasing intertube interactions.
4. Conclusions
The electronic structures of the doublewall heteronanotubes near the Fermi level are dominated by the electrons of carbon atoms; the band structure of the armchair DWHNTs is difficult to modulate with changing intertube distance. However, either changing intertube distance or imposing electric field is the efficient way to modulated the band structure of zigzag DWHNTs. Our results suggest an interesting avenue of exploring novel heterostructure of CNT@BNNT for potentially important applications in CNT@BNNTbased nanodevices.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
This project was supported by the Natural Science Foundation of China (Grant no. 51402251), the Natural Science Foundation of Jiangsu Province of China (Grant no. BK20140471), and Talent Introduction Project of Yancheng Institute of Technology (nos. XKR2011009 and XKR2011001).
References
 C. R. Dean, A. F. Young, I. Meric et al., “Boron nitride substrates for highquality graphene electronics,” Nature Nanotechnology, vol. 5, no. 10, pp. 722–726, 2010. View at: Publisher Site  Google Scholar
 D. Usachov, V. K. Adamchuk, D. Haberer et al., “Quasifreestanding singlelayer hexagonal boron nitride as a substrate for graphene synthesis,” Physical Review B, vol. 82, no. 7, Article ID 075415, 2010. View at: Publisher Site  Google Scholar
 G. Giovannetti, P. A. Khomyakov, G. Brocks, P. J. Kelly, and J. Van Den Brink, “Substrate induced band gap in graphene on hexagonal boron nitride: Ab initio density functional calculations,” Physical Review B, vol. 76, no. 7, Article ID 073103, 2006. View at: Publisher Site  Google Scholar
 J. Sławińska, I. Zasada, and Z. Klusek, “Energy gap tuning in graphene on hexagonal boron nitride bilayer system,” Physical Review B, vol. 81, no. 15, Article ID 155433, 2010. View at: Publisher Site  Google Scholar
 A. Ramasubramaniam, D. Naveh, and E. Towe, “Tunable band gaps in bilayer grapheneBN heterostructures,” Nano Letters, vol. 11, no. 3, pp. 1070–1075, 2011. View at: Publisher Site  Google Scholar
 R. Nakanishi, R. Kitaura, J. H. Warner et al., “Thin singlewall BNnanotubes formed inside carbon nanotubes,” Scientific Reports, vol. 3, article 1385, 2013. View at: Publisher Site  Google Scholar
 A. Gomathi, M. Ramya Harika, and C. N. R. Rao, “Urea route to coat inorganic nanowires, carbon fibers and nanotubes by boron nitride,” Materials Science and Engineering A, vol. 476, no. 12, pp. 29–33, 2008. View at: Publisher Site  Google Scholar
 M. Das, A. K. Basu, S. Ghatak, and A. G. Joshi, “Carbothermal synthesis of boron nitride coating on PAN carbon fiber,” Journal of the European Ceramic Society, vol. 29, no. 10, pp. 2129–2134, 2009. View at: Publisher Site  Google Scholar
 L. Chen, H. Ye, Y. Gogotsi, and M. J. McNallan, “Carbothermal synthesis of boron nitride coatings on silicon carbide,” Journal of the American Ceramic Society, vol. 86, no. 11, pp. 1830–1837, 2003. View at: Publisher Site  Google Scholar
 S. Li, Y. F. Wu, W. Liu, and Y. H. Zhao, “Control of band structure of van der Waals heterostructures: silicene on ultrathin silicon nanosheets,” Chemical Physics Letters, vol. 609, pp. 161–166, 2014. View at: Publisher Site  Google Scholar
 P. Avouris, R. Martel, V. Derycke, and J. Appenzeller, “Carbon nanotube transistors and logic circuits,” Physica B: Condensed Matter, vol. 323, no. 1–4, pp. 6–14, 2002. View at: Publisher Site  Google Scholar
 C. L. Phillips, C. S. Yah, S. E. Iyuke, K. Rumbold, and V. Pillay, “The cellular response of Saccharomyces cerevisiae to multiwalled carbon nanotubes (MWCNTs),” Journal of Saudi Chemical Society, vol. 19, no. 2, pp. 147–154, 2015. View at: Publisher Site  Google Scholar
 K. Chikkadi, M. Muoth, W. Liu, V. Maiwald, and C. Hierold, “Enhanced signaltonoise ratio in pristine, suspended carbon nanotube gas sensors,” Sensors and Actuators, B: Chemical, vol. 196, pp. 682–690, 2014. View at: Publisher Site  Google Scholar
 A. Freitas, S. Azevedo, and J. R. Kaschny, “Effects of a transverse electric field on the electronic properties of single and multiwall BN nanotubes,” Solid State Communications, vol. 153, no. 1, pp. 40–45, 2013. View at: Publisher Site  Google Scholar
 C.W. Chen, M.H. Lee, and S. J. Clark, “Band gap modification of singlewalled carbon nanotube and boron nitride nanotube under a transverse electric field,” Nanotechnology, vol. 15, no. 12, pp. 1837–1843, 2004. View at: Publisher Site  Google Scholar
 P. Ordejón, E. Artacho, and J. M. Soler, “Selfconsistent orderN densityfunctional calculations for very large systems,” Physical Review B, vol. 53, no. 16, Article ID R10441, 1996. View at: Publisher Site  Google Scholar
 D. SánchezPortal, P. Ordejón, E. Artacho, and J. M. Soler, “Densityfunctional method for very large systems with LCAO basis sets,” International Journal of Quantum Chemistry, vol. 65, no. 5, pp. 453–461, 1997. View at: Publisher Site  Google Scholar
 J. P. Perdew, K. Burke, and M. Ernzerhof, “Generalized gradient approximation made simple,” Physical Review Letters, vol. 77, no. 18, pp. 3865–3868, 1996. View at: Publisher Site  Google Scholar
 H. J. Monkhorst and J. D. Pack, “Special points for Brillouinzone integrations,” Physical Review B, vol. 13, no. 12, pp. 5188–5192, 1976. View at: Publisher Site  Google Scholar  MathSciNet
 B. Delley, “An allelectron numerical method for solving the local density functional for polyatomic molecules,” The Journal of Chemical Physics, vol. 92, no. 1, pp. 508–517, 1990. View at: Publisher Site  Google Scholar
 B. Delley, “From molecules to solids with the DMol^{3} approach,” Journal of Chemical Physics, vol. 113, no. 18, pp. 7756–7764, 2000. View at: Publisher Site  Google Scholar
 J. P. Perdew and Y. Wang, “Accurate and simple analytic representation of the electrongas correlation energy,” Physical Review B, vol. 45, no. 23, pp. 13244–13249, 1992. View at: Publisher Site  Google Scholar
 S. Li, Y. Wu, Y. Tu et al., “Defects in silicene: vacancy clusters, extended line defects, and diadatoms,” Scientific Reports, vol. 5, article 7881, 2015. View at: Publisher Site  Google Scholar
 W. Liu, A. Tkatchenko, and M. Scheffler, “Modeling adsorption and reactions of organic molecules at metal surfaces,” Accounts of Chemical Research, vol. 47, no. 11, pp. 3369–3377, 2014. View at: Publisher Site  Google Scholar
 W. Liu, S. N. Filimonov, J. Carrasco, and A. Tkatchenko, “Molecular switches from benzene derivatives adsorbed on metal surfaces,” Nature Communications, vol. 4, article 2569, 2013. View at: Publisher Site  Google Scholar
 W. Liu, J. Carrasco, B. Santra, A. Michaelides, M. Scheffler, and A. Tkatchenko, “Benzene adsorbed on metals: concerted effect of covalency and van der Waals bonding,” Physical Review B, vol. 86, no. 24, Article ID 245405, 2012. View at: Publisher Site  Google Scholar
 J. Yuan and K. M. Liew, “Structural stability of a coaxial carbon nanotube inside a boronnitride nanotube,” Carbon, vol. 49, no. 2, pp. 677–683, 2011. View at: Publisher Site  Google Scholar
 V. Zólyomi and J. Kürti, “Firstprinciples calculations for the electronic band structures of small diameter singlewall carbon nanotubes,” Physical Review B, vol. 70, no. 8, Article ID 85403, 2004. View at: Publisher Site  Google Scholar
 S. V. Tishchenko, “Electronic structure of zigzag carbon nanotubes,” Low Temperature Physics, vol. 32, no. 10, pp. 953–956, 2006. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2015 Xueran Liu et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.